Assembling of Amphiphilic Highly Branched Molecules in
Maryna Ornatska, Sergiy Peleshanko, Kirsten L. Genson, Beth Rybak,
Kathy N. Bergman, and Vladimir V. Tsukruk*
Contribution from the Materials Science and Engineering Department, Iowa State UniVersity,
Ames, Iowa 50011
Received January 7, 2004; E-mail: firstname.lastname@example.org
Abstract: We found that the amplification of weak multiple interactions between numerous peripheral
branches of irregular, flexible, polydisperse, and highly branched molecules can facilitate their self-assembly
into nanofibrillar micellar structures at solid surfaces and the formation of perfect long microfibers in the
course of crystallization from solution. The core-shell architecture of the amphiphilic dendritic molecules
provides exceptional stability of one-dimensional nanofibrillar structures. The critical condition for the
formation of the nanofibrillar structures is the presence of both alkyl tails in the outer shell and amine
groups in the core/inner shell. The multiple intermolecular hydrogen bonding and polar interactions between
flexible cores stabilize these nanofibers and make them robust albeit flexible. This example demonstrates
that one-dimensional supramolecular assembling at different spatial scales (both nanofibers and microfibers)
can be achieved without a tedious, multistep synthesis of shape-persistent molecules.
Dendritic molecules are long thought as a promising building
block for the interfacial organic assemblies for organized
templates and surface nanostructures with tunable properties.1-3
The variation of hydrophobic and hydrophilic interactions by
changing the composition of terminal branches and cores of
these treelike molecules is considered to be a powerful tool for
inducing organized supramolecular structures at surfaces and
interfaces.1,4-9 Because of architectural symmetry, a vast
majority of dendritic molecules studied to date possess globular
or near globular shapes in solution, in bulk, and at weakly
interacting interfaces.1,2,5,10,11 Only specially designed dendritic
molecules with peculiar architectures usually related to sterically
asymmetric fragments were shown to be capable of forming
self-assembled one-dimensional supramolecular structures such
as rods, fibers, ribbons, and helices, all shapes with a special
interest for nanotechnology. The chemical architectures suc-
cessfully used for these arrangements included shape-persistent
planar dendrimers, hairy rod and discotic polymers, rod-coils,
and tapered molecules.1,2,12-14 A proper combination of steric
constraints, stacking interactions, internal rigidity, and hydrogen
bonding is postulated to be critical for precise assembly of these
shape-persistent molecules into large-scale, uniform, one-
dimensional supramolecular structures in solution, in bulk state,
and at interfaces.
The self-organization of long (several centimeters) fibers via
noncovalent synthesis of low molar weight compounds com-
posed of various amphiphiles from amino derivatives, with
fluorinated chains, and phospholipids was reported.15,16 Stupp
et al. developed a synthetic strategy that included different
combinations of rod segments with precisely placed functional
groups and a variety of branched terminations to assemble
organized structures via balanced steric and intermolecular
interactions (rod-dendron molecules).17 The variation of the
chemical composition, the symmetry of molecules, and the
generation of the dendron blocks resulted in the formation of
cubic, lamellar, and cylindrical microstructures in the bulk state
with occasional assembly in long, uniform one-dimensional
ribbons and fibers. It is widely accepted that a precise “match-
(1) Dendrimers and Other Dendritic Polymers; Frechet, J. M. J., Tomalia, D.
A., Eds.; Wiley & Sons: London, 2002.
(2) (a) Sheiko, S. S.; Moller, M. Chem. ReV. 2001, 101, 4099. (b) Percec, V.;
Cho, W. D.; Ungar, G. J. Am. Chem. Soc. 2000, 122, 10273.
(3) (a) Tsukruk, V. V. Prog. Polym. Sci. 1997, 22, 247. (b) Tsukruk, V. V.
AdV. Mater. 2001, 13, 95. (c) Luzinov I.; Minko, S.; Tsukruk, V. V. Prog.
Polym. Sci. 2004, 29, 635.
(4) (a) Brunsveld, L.; Folmer, J.; Meijer, E. W.; Sibesma, R. Chem. ReV. 2001,
101, 4071. (b) Zeng, F.; Zimmerman, S. C. Chem. ReV. 1997, 97, 1681.
(5) Tsukruk, V. V.; Rinderspacher, F.; Bliznyuk, V. N. Langmuir 1997, 13,
(6) Weener, J.-W.; Meijer, E. W. AdV. Mater. 2000, 12, 741.
(7) Jonkheim, P.; Hoeben, F. J.; Kleppinger, R.; van Herrikhuyzen, J.;
Schnenning, A. P.; Meijer, E. W. J. Am. Chem. Soc. 2003, 125, 15941.
(8) Sui, G.; Micic, M.; Huo, Q.; Leblanc, R. M. Langmuir 2000, 16, 7847.
(9) (a) Lee, M.; Kim, J.-W.; Peleshanko, S.; Larson, K.; Yoo, Y.; Vaknin, D.;
Markutsya, S.; Tsukruk, V. V. J. Am. Chem. Soc. 2002, 124, 9121. (b)
Tsukruk, V. V.; Luzinov, I.; Larson, K.; Li, S.; McGrath, D. V. J. Mater.
Sci. Lett. 2001, 20, 873.
(10) Tsukruk, V. V. AdV. Mater. 1998, 10, 253.
(11) (a) Tsukruk, V. V.; Shulha, H.; Zhai, X. Appl. Phys. Lett. 2003, 82, 907.
(b) Shulha, H.; Zhai, X.; Tsukruk, V. V. Macromolecules 2003, 36, 2825.
(12) (a) Zubarev, E. R.; Pralle, M. U.; Sone, E. D.; Stupp, S. I. J. Am. Chem.
Soc. 2001, 123, 4105. (b) Zubarev, E. R.; Pralle, M. U.; Li, L. M.; Stupp,
S. I. Science 1999, 283, 523. (c) Won, Y. Y.; Davis, H. T.; Bates, F. S.
Science 1999, 283, 960. (d) Djalali, R.; Li, S.-Y.; Schmidt, M. Macromol-
ecules 2002, 35, 4282.
(13) Loi, S.; Butt, H.; Wiesler, U.; Mullen, K. Chem. Commun. 2000, 13, 1169.
(14) Liu, D.; Zhang, H.; Grim, P. C.; De Feyter, S.; Wiesler, U.; Berresheim,
A.; Muellen, K.; De Schryver, F. C. Langmuir 2002, 18, 2385.
(15) Furhhop, J. H.; Helfrich, W. Chem. ReV. 1993, 93, 1565.
(16) Menger, M.; Lee, S.; Tao, X. AdV. Mater. 1995, 7, 669.
(17) (a) Pralle, M. U.; Whitaker, C. M.; Braun, P. V.; Stupp, S. I. Macromol-
ecules 2000, 33, 3550. (b) Lecommandoux, S.; Klok, H. A.; Sayar, M.;
Stupp, S. I. J. Polym. Sci., Part A: Polym. Chem. 2003, 41, 3501.
Published on Web 07/09/2004
10.1021/ja0498944 CCC: $27.50 © 2004 American Chemical Society J. AM. CHEM. SOC. 2004, 126, 9675-9684 9 9675
ing” of directional intermolecular interactions and steric con-
straints is required to facilitate long-range one-dimensional
supramolecular assembly of organic and polymeric molecules.
From this standpoint, the assembly of organized supramolecular
structures from irregular, flexible, dendritic molecules could be
Indeed, there are very few reports on the formation of the
organized nanostructures from highly branched (hyperbranched)
molecules composed of irregular, random branched fragments
with the degree of branching well below that observed for ideal
dendritic architecture.18 Because of their irregular architecture,
poorly defined shape, and higher polydispersity, they are not
expected to form regular supramolecular structures, let alone
one-dimensional nanostructures, and are usually considered as
good candidates for the applications when no precise structural
organization and precisely placed functionalities are required.19-22
However, in this report we demonstrate that multiple weak
intermolecular interactions among irregular, highly branched,
and polydisperse molecules which are flexible and symmetrical
can facilitate their assembly into remarkably well-ordered, one-
dimensional supramolecular structures such as long micro- and
nanofibers. We suggest that such an unexpected behavior is
facilitated by a balance of intermolecular and interfacial
interactions caused by appropriate distribution of different
functional groups in the outer shell and the inner core of these
highly branched molecules. To the best of our knowledge, this
is a first example of uniform one-dimensional supramolecular
structures assembled from irregular, highly branched molecules.
Results and Discussion
Chemical Modification and Characterization. Highly
branched polyester core with hydroxyl terminal groups synthe-
sized by a “one-pot” approach with the presence of active core
monomers (so-called hyperbranched molecules of fourth genera-
tion) was obtained from Perstorp Polyols and went via the
purification and fractionation procedures before further chemical
modification (see Supporting Information).23 The esterification
of hyperbranched cores was conducted according to Scheme 1
as suggested in the literature.24,25
Final and all intermediate compounds presented in this
scheme were completely characterized by FTIR, GPC, 1H NMR,
and 13C NMR (see Supporting Information for details). The
degree of branching was calculated using integrated intensities
of the 13C NMR peaks assigned to different monomeric units,
according to the procedure described previously by Hult et al.26
According to this approach, quaternary carbons of the dendritic,
linear, and terminal units can be distinguished by the chemical
shifts of 46.91, 48.93, and 50.92 ppm (Figure 1).
The degree of polymerization was estimated from 1H NMR
and 13C NMR data as well, according to the procedure suggested
by Zagar.27 This analysis indicated that the chemical composi-
tion and the branching structure of the core polyester BH40-pr
(Scheme 1) were close to the literature data for commercial
polyester Boltorn H40.26,27 According to these calculations the
degree of branching of the hyperbranched core after purification
was 40%; the average number of monomeric units (the degree
of polymerization) was 60, and the number average molecular
weight was 7800.
The number of alkyl groups in molecule 3 was determined
from 13C NMR spectra using the ratio of the integral intensities
of the peaks of the methyl group of the palmitic acid group
(14.3 ppm) and